is doping of lifepo4 possible ? desirable ?· possible ? desirable ? a. mauger, c.m. julien, k....
Post on 15-Sep-2018
Embed Size (px)
Is doping of LiFePO4 possible ? Desirable ?
A. Mauger, C.M. Julien, K. Zaghib,
Sorbonne universit, Univ. Paris 06, France
IREQ, 1800 boulevard Lionel-Boulet, Varennes, QC, Canada J3X 1S1
understand the electronic transport of LiFePO4 (LFP) d-electrons responsible for e- transport AND magnetism
Both must be described self-consistently In relation to the electronic structure
Is doping possible (enough to make LFP metallic) ?
Is it desirable ???
orthorhombic olivine structure (Pnma) distorted hexagonal close-packed
framework containing Fe2+ ions
layers of edge-sharing FeO6 octahedra layers are separated by PO4 tetrahedra.
Crystallo-chemistry of LiFePO4 (triphylite)
a=10.3375 , b=6.0112 , c=4.6950
a=9.7599 , b=5.7519 , c=4.7560 .
A.K. Padhi et al. JECS 144, 1188 (1997). N. Ravet et al. J Pw S 97-98, 503 (2001). N. Ravet US Patent 6,962,666 (2005).
Zhou, F.; Cococcioni, M.; Kang, K.; Ceder, G. Electrochem. Commun. 2004, 6, 1144.
-10.0 -8.0 -6.0 -4.0 -2.0 0.0 2.0 4.0 6.0
Fe2+ in (eg)2(tg)3tg spin S=2 4
(R) = (1 R)2 /2R
(R)h[ ]n h
n=2 (instead of 1/2)
The energy gap is HUGE: 3.84 eV LFP is IONIC, not a semiconductor
Formation of small polaron
Ea=0.6 eV characteristics
of Fe-phosphate glasses: xP2O5 (1-x)FeO (50-x)FeO 50 P2O5 xBaO
Etc. Murawski et al. J. Mater. Sci. 1982, 17, 2155. Solid State Ionics 2003, 157, 293 and references therein
Mott formula: wave function decay for iron ion is = 1.5 -1
Fe-Fe distance is R=3.87 . electronic frequency is e = 1015 Hz Ea =0.62 eV: barrier energy to overcome to jump on next site c= [Fe3+]/[Fe2++Fe3+] = 3.510-3
=c(1c)e2eRkT exp(2R)exp EakT
' ( (
* + +
0 50 100 150 200 250 300 350
(Magnetic) polaron in LiFePO4
Fe3+ (tg )3(eg )2
Fe2+ (tg )3(eg )2tg
What does the Curie-Weiss law tell us at T>TN ? )1( += SSg Beff
eff2=(1-c)[(Fe2+)]2+c(pol)2-8c[(Fe2+)]2 eff=5.36, pol = (8*2+5/2)*2 =37 c = 3x10-3
Magnetic polaron in LiFePO4
spin only value (quenched)
Theretical value for Fe2+(S=2): 4.90B
Gd3+ ion or O vacancy
Case of a semiconductor: EuO (ferromagnet, Tc=69 K)
Case of doped EuO In the paramagetic phase:
Formation of a polaron
Case of doped EuO In the ferromagnetic phase:
Eu2+ and Gd3+ carry a spin S=7/2
0 100 200 300 400
EuO Mauger, A.; Godart, C. Solid State Commun. 1980, 35, 735.
Polaronic regime Ea=0.6 eV: energy to send
the bound electron To the conduction band
Doping by substitution of Fe2+ by Mn+ (n2) is not
possible because LFP is too ionic: HOPPING transport, i.e. not driven by ionization of
electrons of bound polarons)
Nb5, Zr4, Ti4, Cr3+, V5 combined neutron and X-ray diffraction studies locate the supervalent-cation dopants (Zr,Nb,Cr) on Li, and charge compensation assumed by Li vacancies: M. Wagemaker, B.L. Ellis, D. Ltzenkirchen-Hecht, F.M. Mulder, L. Nazar, Chem. Mater. 2008, 20, 63136315.
Any other claim results from artifacts (metal Nb, Zr, impurities at the surface)
Doping is not to be confused with surface modifications
Surface coating by conductive carbon is the best solution since 2001. Alternative: conductive polymer
Since the limit of solution of dopant such as Nb, Zr, Cr, Ti, V etc is small (3%), the excess may form a metal coat at the surface (uncontrolled + massy; should be avoided).
Coating with Fe2P: efficient only on a short term basis: Fe2P dissolves into the electrolyte: reduces the calendar life: PROHIBITED !!
Doping with Mg ??
If Mg is in subsitution to Fe: isovalent (2+): no doping in any other case, the channels are blocked: If Mg in substitution on Li (J. Song, Y. Zhang, G. Shao, J. Nanomat. (2013) Article ID 687501): damageable Ab initio calculations: antisite (Mg on Li site + Li on Fe site) H. Zhang et al. Appl. Phys. A 104 (2011) 529
Li-rich: LiFePO4 + x Li3PO4 does not work Li-poor: Li1-2xFexFePO4, i.e. FeLi + 2V/Li does not work
P. Axmann, C. Stinner, M. Wolfhart-Mehrens, A. Mauger, F. Gendron, C.M. Julien, Chem. Mater. 21, 1636 (2009).
Such a doping is impossible
Doping by deviation from stoichiometry ?
F-1 doping X.Z. Liao, Y.S. He, Z.F. Ma, X.M. Zhang, L. Wang, J. Power Sources
174 (2007) 720 assume that 3(F-) substitute for (PO4)3-, very unlikely: computations suggest that O tends to be replaced by Cl- [M.E. Arroyoy de Dompablo, U. Amador, J.M. Tarascon, J. Power Sources 174 (2007) 1251] the results are not as good as undoped C-LiFePO4.
Cl- doping Cl- doped C-LFP has a cacacity 90 mAh/g at rate 20C but tests on few
cycles only, and concentration of Cl- is unknown ! [C.S. Sun, Y. Zhang, X.J. Zhang, Z. Zhou, J. Power Sources 195 (2010) 3680].
In any case it means a deformation of the PO43- ions
(confirmed by the changes in P-O distances by Cl-doping)
What if the PO4 phosphate is de-stabilized by anion doping so that the material reduces to a simple
transition metal oxide ???
Two major consequences
Lost of thermal stability Tendency to loose oxygen that will migrate to the carbon
electrode, and C+O2 --> CO2 exothermic reaction: thermal runaway: we have lost SAFETY
R. Huggins J. Electrochem. Soc. 160 (2013) A3001
Do you really want an unsafe battery ?
R. Huggins J. Electrochem. Soc. 160 (2013) A3001
Conclusion Self-consistent quantitative analysis of both electronic and magnetic properties show that LiFePO4 is a truly ionic material.
The small polaron is a new kind of magnetic polaron that must be distinguished from the other kinds of magnetic polarons investigated before in magnetic (not so ionic) semiconductors. Consequence: cation doping is not possible. Doping by deviation from stoichiometry is not possible Anion doping is possible, BUT not desirable: no evident improvement vs. un-doped C-LFP, plus risks to loose thermal stability, and loss of safety (check equilibrium pressure of oxygen !!)